Research Article  Open Access
Study on Dynamic Mechanical Properties of Full Tailings Cemented Backfilling Impacted by CementSand Ratio
Abstract
In order to study the effect of cementsand ratio on the dynamic mechanical properties of the full tailings cemented backfilling, three sets of full tailings cemented backfilling specimens with different cementsand ratios were prefabricated. The uniaxial impact of the prefabricated specimens was performed by the Ф50 mm SHPB test system. Test results showed that full tailings cemented backfilling had strong reflection and damping effects on elastic wave propagation. At lower strain rates, specimens presented strength hardening, and at higher strain rates, the test specimens presented rapidsoftening strength; the strengthhardened specimen reached the peak stress at 40 μs, and the softening specimen reached the peak stress at about 18 μs; with the increase of strain rate, dynamic compressive strength, growth factor of dynamic strength, peak strain, and dynamicstatic strain ratio of specimens increased totally. When the cementsand ratio increased, ultimate dynamic compressive strength, limit dynamic strength growth factor, and ultimate peak strain of the specimen were higher; at the same strain rate, with the increase of cement content, the dynamic compressive strength, dynamic strength growth factor, and dynamicstatic strain ratio of the test piece all decreased. The failure mode of the specimen was crushing failure. Under the same strain rate, when the cement content decreased, there was a higher damage degree of specimens.
1. Introduction
Filling mining method has the advantages of high recovery rate, high safety, and low pollution degree, which has been widely used in underground mines at home and abroad [1–3]. The full tailings cemented backfilling is a commonly used filling material in metal mine. According to the characteristics of the mining process, it is vital to grasp the dynamic mechanical characteristics of the cemented backfilling for filling mining technology [4]. Many scholars have conducted relevant research studies on the dynamic and static mechanical properties of full tailings cemented backfilling. Xue [5] carried out quasistatic uniaxial compression and splitting tests on the full tailings cemented backfilling of Huangmeiling Mine and studied the quasistatic mechanical properties of the full tailings cemented backfilling. Dong [6] conducted an onsite blasting vibration test on the backfill body and studied the damage law of the backfill under blasting vibration. Zhixiang et al. [7] analyzed the deformation and damage characteristics of different proportions of backfills and established the damage of different filling backfills. Structural equations were studied to investigate the deformation, damage, and energy release of different filling ratios. However, there are certain limitations in these studies. For instance, the cementsand ratio of the backfills was relatively single, and the dynamic load was small in the literature [4–6]. The literature [7] could not reflect mechanical properties of the full tailings cemented backfilling at high strain rates. In this paper, the relationship between the dynamic stressstrain rate of the material was studied by using the splitHopkinson pressure bar (SHPB) [8–10]. In order to study the effect of cementsand ratio on the dynamic mechanical properties of the full tailings cemented backfilling, three sets of full tailings cemented backfilling specimens with different cementsand ratio were prefabricated, and uniaxial impact tests were performed on precast specimens by Ф50 mm SHPB test system, so as to investigate the dynamic mechanical properties of specimens at high strain rates.
2. SHPB Test Principle
The splitHopkinson pressure bar (SHPB) was developed by Hopkinson [11] and further improved by Kolsky [12] to test the strength of materials at high strain rates from 101 to 104 s. Li et al. [13] developed a coneshaped striker which could produce a wellrepeatable and slowrising halfsine wave to reduce high frequency oscillations, minimize the dispersion effect, and overcome the premature failure for brittle materials. Due to its easy operation and relatively accurate results, it was suggested as a standard testing method for dynamic properties of rock materials including dynamic compressive and tensile strengths, as well as mode I fracture toughness by the International Society for Rock Mechanics [14].
Figure 1 is a schematic diagram of the SHPB compression test principle. The test system consists of a launcher, a punch, an entrance rod (density: 7.810 g/cm^{3}, elastic wave velocity: 5410 m/s, and wave impedance: 4.23 × 107 kg·m^{−2}·s^{−1}), and transmissive rod, etc. The test sample was sandwiched between the incident rod and the transmissive rod. The punch hit the incident rod under the action of high pressure, and a stress pulse () was generated at the end of the incident rod. Under the condition of onedimensional stress propagation, the stress pulse, namely, the elastic stress incident wave, propagated forward at the wave velocity C_{0} in the entrance rod. The reflection stress pulse () and a transmission stress pulse () were generated in the entrance rod and the transmission rod after contacting the sample. Besides, the incident strain () and the reflection strain () were generated at the end of the specimen, and the transmission strain () was produced by the transmitted rod simultaneously. The dynamic stress (), strain rate (), and strain () of the specimen were related to each strain as shown in the following equations:where is the crosssectional area of the incident rod; is the crosssectional area of the specimen; is the elastic modulus of the plunger; and is the thickness of the specimen.
According to the onedimensional stress assumption, when the sample stress reaches the equilibrium, Equation (4) is obtained as
Subsequently, Equation (1)∼(3) can be simplified as
3. Test Materials and Equipment
Full tailings of an iron ore mine in Hebei Province was taken as the aggregate of samples. The proportion of particles below 0.075 mm in tailings was 69.1%, and the median diameter d_{50}(mm) was 0.049. 525# Portland cement was used as a gelling agent whose mass concentration was 72%. The cementsand ratio was 1 : 4, 1 : 6, and 1 : 8, respectively. Figure 2 shows a sketch of the specimen. The basic physical and mechanics parameters of the full tailings cement block are shown in Table 1.

4. Mechanical Test Results and Analysis
In rock dynamics, the growth factor of dynamic strength K and the dynamicstatic strain ratio are often used to quantify the strength variation of the specimen under dynamic and static load conditions [15]. Expressions of K and are given by Equations (6) and (7) as follows. These two indicators were also used to assist the analysis in this test result:where is the growth factor of dynamic strength; is the dynamicstatic strain ratio; is the dynamic compressive strength of the sample; is the static compressive strength of the sample; and and are the maximum strains of the sample under dynamic load and static load, respectively.
4.1. SHPB Original Waveform
The typical incident wave, reflected wave, and transmitted wave waveform obtained by the test recorder are shown in Figure 3. From the original waveform diagram, it can be seen basically that the amplitude of the incident wave and the reflected wave is approximately equal with opposite directions, while the amplitude of the transmitted wave is relatively small. Wave impedance theory can explain this phenomenon clearly [16]. When an elastic wave was incident on a lowwave impedance material from a highwave impedance material, the reflected wave and the incident wave were different in sign, and the transmitted wave had a smaller magnitude of stress amplitude than that of the incident wave. Namely, the stress wave was transmitted from the hard material to the soft material. The incident wave impedance of the rod (4.23 × 107 kg·m^{−2}·s^{−1}) was much larger than that of the full tail cement specimen, while the stress amplitude of transmitted wave was much smaller than that of the incident wave. Figure 3 illustrates that full tailings cemented backfilling test specimen has a strong damping effect on the elastic wave propagation.
4.2. Mechanical Test Results and Analysis
4.2.1. Test Results
The uniaxial impact test has been divided into 3 groups and conducted for 36 times, which obtained 30 groups of ideal test results. The partial results of mechanical tests are shown in Table 2. Typical stressstrain curves in the tests are shown in Figure 4.

4.2.2. Dynamic Properties of Specimens
The test results in Table 2 were extracted and fitted, as shown in Figures 5–8. The relationship between the dynamic compressive strength and the strain rate of proportioned specimens has a similar pattern. Test results of specimens in group A are analyzed as an example.(1)The stressstrain curve of specimens was different from general brittle materials [17, 18]. The stressstrain curve generally had several stress peaks. At a lower strain rate, the specimen presented dynamic strength hardening. Namely, after reaching stress A, a small part of the specimen began to fail and the stress began to decrease slightly. Meanwhile, the other part of the microcracks was gradually compacted and the stress gradually rose again to the true peak value of stress B. After several “damagecompacting” oscillations, the specimen finally failed, as shown in Figure 4(a). At higher strain rates, the specimen showed a rapid softening of the dynamic strength [19]. Namely, under the impact load, when the stress reached the stress peak quickly, most of the specimen began to break with the rapid decrease of the stress. At the same time, compaction process occurred in the other parts, and the stress rose slightly. After several waveform oscillation processes, the sample was damaged finally, as shown in Figure 4(b). From Table 2, it can be seen that all strengthhardened specimens reach peak stress after 40 μs, and all strength accelerating softening specimens reach peak stress around 18 μs.(2)From Table 2, it can be seen that, the dynamic compressive strength increases with the increase of the strain rate in the initial stage. When the strain rate reaches 266 s^{−1}, the dynamic compressive strength reaches the maximum, of 17.27 MPa, while with the increasing strain rate, it decreases. The stressstrain rate fitting curve is shown in Figure 5, and the fitting relationship is obtained in the following equation:(3)Figure 6 illustrates that the growth factor of dynamic strength K_{A} increases significantly with the increasing strain rate. K_{Amax} is 6.28, which means that the dynamic compressive strength is 6.28 times than the static compressive strength, while the general dynamic growth factor of the rock is only 1.2–2.5 or so [20]. The fitting curve of dynamic strength growth factor and strain rate is shown in Figure 6, and the fitting relationship is described in the following equation:(4)Figure 7 indicates that as the strain rate increases, the peak strain of all specimens has a linear increasing trend with the limit peak strain of 0.0274. Comparing Table 1 and Table 2, maximum dynamic strain is less than the maximum quasistatic strain, and the dynamicstatic strain ratio increases with the increase of strain rate, = 0.5. Besides, the fitting curve of maximum dynamicstatic strain ratio and strain rate is shown in Figure 8, and the fitting relationship is described in the following equation:
4.2.3. Effect of CementSand Ratio on Dynamic Mechanical Properties of Specimen
(1)Figure 5 indicates that the greater the cement content (cementsand ratio), the greater the ultimate dynamic compressive strength of the specimen and the greater the strain rate corresponding to ; at the same strain rate, the dynamic compressive strength of the specimen decreases with increasing cement content. Figure 6 shows that the larger the cement content, the larger the growth factor of limit dynamic strength K_{max} of the specimen and the larger the strain rate corresponding to K_{max}; at the same strain rate, the K value of the specimen decreases with the increasing cement content.(2)Figure 7 shows that the larger the cement content, the larger the limit dynamic strain of the specimen and the greater the strain rate corresponding to ; at the same strain rate, the peak strain of the specimen increases as the cement content increases. Figure 8 shows that the greater the cement content, the smaller the maximum dynamic and static strain ratio of the specimen; at the same strain rate, the dynamic and static strain ratio of the specimen decreases as the cement content increases.(3)As shown in Figure 9, as a whole, the failure mode of the test block is crush damage, which is similar to the damage form of lowstrength concrete [17]. At the same strain rate, the lesser the cement content, the higher the damage degree of the test block. Taking the strain rate of 56s^{−1} as an example, when cementsand ratio was 1 : 4, the specimen was situated in a critical failure state, and the specimen presented chapping failure in the axial direction (Figure 9(a)); when the cementsand ratio was 1 : 6, the number of fragments in specimens relatively increased and a small amount of powder was presented (Figure 9(b)). When the cementsand ratio was 1 : 6, most of the specimens were completely pressed into powders with few small particles (Figure 9(c)).
(a)
(b)
(c)
5. Conclusions
In order to study the effect of cementsand ratio on the dynamic mechanical properties of the full tailings cemented backfilling, three sets of full tailings cemented backfilling specimens with different cementsand ratio were prefabricated. Uniaxial impact tests were performed on precast specimens by the Ф50 mm SHPB test system. Conclusions are obtained as follows:(1)According to the original waveform diagram of SHPB, the full tailings cemented backfilling had strong reflection and damping effects on elastic wave propagation.(2)Stressstrain curves of the specimen were divided into two types: hardening and softening. At lower strain rates, specimens presented strength hardening; at higher strain rates, the specimens showed rapidsoftening strength. The strengthhardened specimen reached its peak stress after 40 μs, and the strengthaccelerating softening specimen reached peak stress at about 18 μs; The dynamic compressive strength, growth factor of dynamic strength, peak strain, and dynamicstatic strain ratio of the specimen increased with the increasing strain rate.(3)The higher the cement content (cementsand ratio), the greater the ultimate dynamic compressive strength, the limit dynamic strength growth factor, and the ultimate peak strain of the specimen; at the same strain rate, the dynamic compressive strength, growth factor of dynamic strength, and dynamicstrain ratio of the specimen decreased with increasing cement content. The failure mode of the specimen was crush damage. Under the same strain rate, lesser the cement content, the higher the damage degree of the specimen.
Data Availability
The experimental data used to support the findings of this study are included within the article.
Conflicts of Interest
The authors declare that they have no conflicts of interest.
Acknowledgments
This study was supported by the National Natural Science Foundation of China (Grant nos. 51404305 and 51504286).
References
 F. Yulu, W. Yang, Z. Guohui et al., “Surround rock stability of mined out area under blast loading metal mine pillar robbing,” Explosion and Shock Waves, vol. 33, no. 4, pp. 344–350, 2013. View at: Google Scholar
 Q. Zhang, W. Yang, and X. Wang, “Experiment with filling the stope area with the wet pastelike fly ash material,” Journal of Safety and Environment, vol. 14, no. 5, pp. 70–72, 2014. View at: Google Scholar
 G. Huang, S. J. Cai, Y. D. Zhang, and D. Wu, “Experimental and modeling study on the strength of tailings backfill in underground mine,” Applied Mechanics and Materials, vol. 522–524, pp. 1390–1393, 2014. View at: Publisher Site  Google Scholar
 M. Fall, J. C. Célestin, M. Pokharel, and M. Touré, “A contribution to understanding the effects of curing temperature on the mechanical properties of mine cemented tailings backfill,” Engineering Geology, vol. 114, no. 34, pp. 397–413, 2010. View at: Publisher Site  Google Scholar
 X.L. Xue, A Study of High Density Total Tailings Backfill Technology in Huangmei Phosphorus Mine, Central South University, Changsha, China, 2012.
 K.C. Dong, Research on the Influence and Control Techniques of Blasting Seismic Wave on Backfill, Central South University, Changsha, China, 2010.
 L. ZhiXiang, Li. Xibing, D. Tagen, and C. Ping, “On damage model of cemented tailings backfill and its match with rock mass,” Rock and Soil Mechanics, vol. 27, no. 9, pp. 1442–1446, 2006. View at: Google Scholar
 Z. Zhou, X. Li, Z. Ye, and K. Liu, “Obtaining constitutive relationship for ratedependent rock in SHPB tests,” Rock Mechanics and Rock Engineering, vol. 43, no. 6, pp. 697–706, 2010. View at: Publisher Site  Google Scholar
 H. Meng and Q. M. Li, “Correlation between the accuracy of a SHPB test and the stress uniformity based on numerical experiments,” International Journal of Impact Engineering, vol. 28, no. 5, pp. 537–555, 2003. View at: Publisher Site  Google Scholar
 B. Yang, L. Tang, Y. Liu, Z. Liu, Z. Jiang, and D. Fang, “The deformation measurement and analysis on mesostructure of aluminum foams during SHPB test,” Journal of Testing and Evaluation, vol. 42, no. 3, Article ID 20120254, 2014. View at: Publisher Site  Google Scholar
 B. Hopkinson, “A method of measuring the pressure produced in the detonation of high explosives or by the impact of bullets,” Philosophical Transactions of the Royal Society A: Mathematical, Physical and Engineering Sciences, vol. 213, no. 497–508, pp. 437–456, 1914. View at: Publisher Site  Google Scholar
 H. Kolsky, “An investigation of the mechanical properties of materials at very high rates of loading,” Proceedings of the Physical Society. Section B, vol. 62, no. 11, pp. 676–700, 1949. View at: Publisher Site  Google Scholar
 X. B. Li, T. S. Lok, and J. Zhao, “Dynamic characteristics of granite subjected to intermediate loading rate,” Rock Mechanics and Rock Engineering, vol. 38, no. 1, pp. 21–39, 2005. View at: Publisher Site  Google Scholar
 Z. Zhou, X. Cai, D. Ma, L. Chen, S. Wang, and L. Tan, “Dynamic tensile properties of sandstone subjected to wetting and drying cycles,” Construction and Building Materials, vol. 182, pp. 215–232, 2018. View at: Publisher Site  Google Scholar
 M. Peroni, L. Peroni, and M. Avalle, “High strainrate compression test on metallic foam using a multiple pulse SHPB apparatus,” Journal de Physique IV (Proceedings), vol. 134, pp. 609–616, 2006. View at: Publisher Site  Google Scholar
 J. Dai, Rock Dynamics and Blasting Theory, Press of Metallurgy Industry, Beijing, China, 2002.
 M. R. Mitchell, R. E. Link, S. Wang, M.H. Zhang, and S. T. Quek, “Effect of specimen size on static strength and dynamic increase factor of highstrength concrete from SHPB test,” Journal of Testing and Evaluation, vol. 39, no. 5, Article ID 103370, 2011. View at: Publisher Site  Google Scholar
 J. Liu, J. Xu, and L. Xiaocong, “Experimental study on dynamic mechanical properties of amphibolites under impact compressive loading,” Chinese Journal of Rock Mechanics and Engineering, vol. 28, no. 10, pp. 2113–2120, 2009. View at: Google Scholar
 J. Qu and G. Zou, “A study of the dynamic plane strain fracture toughness of concrete by SHPB,” Key Engineering Materials, vol. 385–387, pp. 21–24, 2008. View at: Publisher Site  Google Scholar
 X. Li, F. Gong, J. Zhao et al., “Test study of impact failure of rock subjected to onedimensional coupled static and dynamic loads,” Chinese Journal of Rock Mechanics and Engineering, vol. 29, no. 2, pp. 251–260, 2010. View at: Google Scholar
Copyright
Copyright © 2018 Shan Yang et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.